# Electronic Supplementary Material (ESI) for ChemComm.
# This journal is © The Royal Society of Chemistry 2021

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_p21c_a
_database_code_depnum_ccdc_archive 'CCDC 2109533'
loop_
_audit_author_name
_audit_author_address
'Philip Yox'
;Iowa State University
United States of America
;
_audit_update_record             
;
2021-09-13 deposited with the CCDC.	2021-11-17 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2018/3
_shelx_SHELXL_version_number     2018/3
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'As30 Au16 Ba8'
_chemical_formula_sum            'As30 Au16 Ba8'
_chemical_formula_weight         6497.78

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Au Au -2.0133 8.8022 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/c'
_space_group_name_Hall           '-P 2ybc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   15.1473(14)
_cell_length_b                   15.2189(14)
_cell_length_c                   10.9542(10)
_cell_angle_alpha                90
_cell_angle_beta                 90.502(2)
_cell_angle_gamma                90
_cell_volume                     2525.1(4)
_cell_formula_units_Z            2
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    59395
_cell_measurement_theta_min      1.90
_cell_measurement_theta_max      29.0

_exptl_crystal_description       block
_exptl_crystal_colour            'metallic silver'
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    8.546
_exptl_crystal_F_000             5404.0
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.03
_exptl_absorpt_coefficient_mu    71.902
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.43
_exptl_absorpt_correction_T_max  0.75
_exptl_absorpt_process_details   SADABS
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'fine-focus sealed tube'
_diffrn_measurement_device_type  'Bruker APEX II CCD area-detector'
_diffrn_measurement_method       'profile data from ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            59395
_diffrn_reflns_av_unetI/netI     0.0462
_diffrn_reflns_av_R_equivalents  0.0904
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_theta_min         1.897
_diffrn_reflns_theta_max         28.998
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             6719
_reflns_number_gt                5386
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
# start Validation Reply Form
_vrf_PLAT112_p21c_a              
;
PROBLEM: ADDSYM Detects New (Pseudo) Symm. Elem        42        100 %Fit  
RESPONSE: Analysis of High Resolution Powder Diffraction confirms P21/c symmetry
;
_vrf_PLAT113_p21c_a              
;
PROBLEM: ADDSYM Suggests Possible Pseudo/New  Space Group    P42/mmc Check 
RESPONSE: Analysis of High Resolution Powder Diffraction confirms P21/c symmetry
;
# end Validation Reply Form 
_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0094P)²+27.8222P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_extinction_coef       0.000063(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         6719
_refine_ls_number_parameters     248
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0496
_refine_ls_R_factor_gt           0.0320
_refine_ls_wR_factor_ref         0.0576
_refine_ls_wR_factor_gt          0.0536
_refine_ls_goodness_of_fit_ref   1.061
_refine_ls_restrained_S_all      1.061
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Au1 Au 0.18576(3) 0.00117(2) 0.67524(4) 0.00399(8) Uani 1 1 d . . . . .
Au2 Au 0.33495(3) 0.34785(2) 0.60876(4) 0.00438(9) Uani 1 1 d . . . . .
Au3 Au 0.93769(3) 0.45235(2) 0.31966(4) 0.00418(9) Uani 1 1 d . . . . .
Au4 Au 0.49777(3) 0.18545(2) 0.81696(4) 0.00446(9) Uani 1 1 d . . . . .
Au5 Au 0.38219(3) 0.61661(3) 0.99417(4) 0.00484(9) Uani 1 1 d . . . . .
Au6 Au 0.15568(3) 0.33480(2) 0.88994(4) 0.00423(9) Uani 1 1 d . . . . .
Au7 Au 0.90032(3) 0.21644(2) 0.50919(4) 0.00408(8) Uani 1 1 d . . . . .
Au8 Au 0.71212(3) 0.39273(3) 0.50840(4) 0.00425(9) Uani 1 1 d . . . . .
Ba1 Ba 0.500000 0.000000 1.000000 0.00381(17) Uani 1 2 d S . P . .
Ba2 Ba 0.000000 0.000000 0.500000 0.00392(17) Uani 1 2 d S . P . .
Ba3 Ba 0.74935(4) 0.24596(4) 0.75305(7) 0.00912(13) Uani 1 1 d . . . . .
Ba4 Ba 0.88567(4) 0.62480(4) 0.50735(7) 0.00917(14) Uani 1 1 d . . . . .
Ba5 Ba 0.36703(4) 0.37843(4) 1.01159(7) 0.01029(14) Uani 1 1 d . . . . .
As1 As 0.18694(7) 0.49467(7) 0.82189(10) 0.0037(2) Uani 1 1 d . . . . .
As2 As 0.93834(7) 0.43770(6) 0.69746(10) 0.0037(2) Uani 1 1 d . . . . .
As3 As 0.55412(7) 0.43718(6) 0.80385(10) 0.0035(2) Uani 1 1 d . . . . .
As4 As 0.24712(7) 0.24901(6) 0.74554(10) 0.0033(2) Uani 1 1 d . . . . .
As5 As 0.43962(7) 0.55529(7) 0.79785(10) 0.0042(2) Uani 1 1 d . . . . .
As6 As 0.14949(7) 0.15741(6) 0.62083(10) 0.0033(2) Uani 1 1 d . . . . .
As7 As 0.99531(7) 0.18136(7) 0.69507(10) 0.0040(2) Uani 1 1 d . . . . .
As8 As 0.87636(7) 0.37816(7) 0.50646(10) 0.0037(2) Uani 1 1 d . . . . .
As9 As 0.59151(7) 0.28279(7) 0.50367(10) 0.0041(2) Uani 1 1 d . . . . .
As10 As 0.30893(7) 0.50467(7) 0.67961(10) 0.0039(2) Uani 1 1 d . . . . .
As11 As 0.34228(7) 0.14995(7) 0.87641(10) 0.0036(2) Uani 1 1 d . . . . .
As12 As 0.99602(7) 0.31090(7) 0.82013(10) 0.0035(2) Uani 1 1 d . . . . .
As13 As 0.21567(7) 0.59652(7) 0.99330(10) 0.0040(2) Uani 1 1 d . . . . .
As14 As 0.49390(7) 0.31357(7) 0.67639(10) 0.0035(2) Uani 1 1 d . . . . .
As15 As 0.31640(7) -0.00249(6) 0.81333(10) 0.0042(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Au1 As15 2.4809(12) . ?
Au1 As6 2.5111(11) . ?
Au1 As13 2.5306(12) 4_565 ?
Au1 As2 2.5410(11) 2_646 ?
Au1 Ba2 3.3923(5) . ?
Au1 Ba5 3.7679(8) 4_565 ?
Au1 Ba3 4.0810(8) 2_646 ?
Au1 Ba4 4.1068(9) 2_646 ?
Au2 As4 2.5125(11) . ?
Au2 As10 2.5415(11) . ?
Au2 As11 2.5488(12) 4_565 ?
Au2 As14 2.5665(11) . ?
Au2 Ba4 3.5895(8) 3_666 ?
Au2 Ba1 3.6172(4) 2_656 ?
Au2 Ba5 3.6383(8) 4_565 ?
Au3 As8 2.5215(11) . ?
Au3 As2 2.5233(11) 3_766 ?
Au3 As1 2.5626(12) 3_666 ?
Au3 As7 2.6050(11) 4_565 ?
Au3 Ba4 3.4299(8) . ?
Au3 Ba4 3.4697(8) 3_766 ?
Au3 Ba2 3.7062(5) 2_655 ?
Au4 As14 2.4848(11) . ?
Au4 As11 2.5081(11) . ?
Au4 As9 2.5262(12) 4_566 ?
Au4 As5 2.5350(11) 2_646 ?
Au4 Ba1 3.4621(5) . ?
Au4 Ba3 3.9883(8) . ?
Au4 Ba5 3.9925(9) 4_565 ?
Au5 As5 2.5070(12) . ?
Au5 As13 2.5407(11) . ?
Au5 As3 2.5414(12) 3_667 ?
Au5 As9 2.5604(11) 2_656 ?
Au5 Ba5 3.6372(8) . ?
Au5 Ba5 3.8004(8) 3_667 ?
Au5 Ba3 3.8839(8) 2_656 ?
Au5 Ba3 4.0136(8) 3_667 ?
Au6 As4 2.4827(11) . ?
Au6 As6 2.5345(12) 4_566 ?
Au6 As12 2.5561(12) 1_455 ?
Au6 As1 2.5896(11) . ?
Au6 Ba4 3.4475(8) 2_646 ?
Au6 Ba5 3.5201(8) . ?
Au6 Ba2 3.6585(4) 2_556 ?
Au7 As8 2.4881(11) . ?
Au7 As13 2.5332(11) 2_646 ?
Au7 As7 2.5396(12) . ?
Au7 As12 2.5721(12) 4_565 ?
Au7 Ba3 3.5601(8) . ?
Au7 Ba2 3.6253(5) 1_655 ?
Au7 Ba3 3.6492(9) 4_565 ?
Au7 Ba4 4.0484(8) 3_766 ?
Au8 As9 2.4775(11) . ?
Au8 As8 2.4978(11) . ?
Au8 As15 2.5608(12) 2_656 ?
Au8 As10 2.6020(12) 3_666 ?
Au8 Ba3 3.5302(8) . ?
Au8 Ba3 3.5532(8) 4_565 ?
Au8 Ba1 3.6045(5) 2_656 ?
Ba1 As14 3.4344(11) 4_566 ?
Ba1 As14 3.4344(11) 2_646 ?
Ba1 As15 3.4376(11) . ?
Ba1 As15 3.4376(11) 3_657 ?
Ba1 As5 3.4989(11) 4_566 ?
Ba1 As5 3.4989(11) 2_646 ?
Ba1 As10 3.5146(11) 4_566 ?
Ba1 As10 3.5146(11) 2_646 ?
Ba1 As3 3.5520(12) 2_646 ?
Ba1 As3 3.5520(12) 4_566 ?
Ba2 As1 3.4536(11) 4_565 ?
Ba2 As1 3.4536(11) 2_546 ?
Ba2 As12 3.4880(11) 4_465 ?
Ba2 As12 3.4880(11) 2_646 ?
Ba2 As7 3.4917(11) 3_656 ?
Ba2 As7 3.4917(11) 1_455 ?
Ba2 As6 3.5448(11) . ?
Ba2 As6 3.5448(11) 3_556 ?
Ba2 As2 3.5637(11) 4_465 ?
Ba2 As2 3.5637(12) 2_646 ?
Ba3 As13 3.5721(13) 2_646 ?
Ba3 As9 3.6577(14) . ?
Ba3 As9 3.6822(13) 4_566 ?
Ba3 As13 3.7043(13) 3_667 ?
Ba3 As10 3.8497(12) 2_646 ?
Ba3 As8 3.8576(13) 4_566 ?
Ba4 As8 3.6094(12) 3_766 ?
Ba4 As2 3.6127(13) . ?
Ba4 As2 3.6262(12) 3_766 ?
Ba4 As6 3.6371(12) 3_666 ?
Ba4 As11 3.7104(12) 2_656 ?
Ba4 As8 3.7561(12) . ?
Ba4 As7 3.8097(14) 2_756 ?
Ba4 As12 3.8399(13) 2_756 ?
Ba5 As6 3.5576(12) 4_566 ?
Ba5 As3 3.6533(13) 3_667 ?
Ba5 As4 3.7027(13) 4_566 ?
Ba5 As5 3.7209(13) 3_667 ?
Ba5 As5 3.7391(13) . ?
Ba5 As3 3.7580(13) . ?
Ba5 As11 3.7967(13) . ?
As1 As10 2.4325(15) . ?
As1 As13 2.4705(15) . ?
As2 As8 2.4588(16) . ?
As2 As12 2.5046(15) . ?
As3 As5 2.4983(14) . ?
As3 As14 2.5096(15) . ?
As3 As15 2.5261(15) 2_656 ?
As4 As6 2.4416(15) . ?
As4 As11 2.5238(15) . ?
As5 As10 2.4789(16) . ?
As6 As7 2.5063(15) 1_455 ?
As7 As12 2.4007(15) . ?
As9 As14 2.4566(15) . ?
As11 As15 2.4512(15) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
As15 Au1 As6 109.74(4) . . ?
As15 Au1 As13 108.64(4) . 4_565 ?
As6 Au1 As13 114.19(4) . 4_565 ?
As15 Au1 As2 104.29(4) . 2_646 ?
As6 Au1 As2 109.20(4) . 2_646 ?
As13 Au1 As2 110.32(4) 4_565 2_646 ?
As15 Au1 Ba2 176.50(3) . . ?
As6 Au1 Ba2 72.06(3) . . ?
As13 Au1 Ba2 72.82(3) 4_565 . ?
As2 Au1 Ba2 72.22(3) 2_646 . ?
As15 Au1 Ba5 73.76(3) . 4_565 ?
As6 Au1 Ba5 65.51(3) . 4_565 ?
As13 Au1 Ba5 76.99(3) 4_565 4_565 ?
As2 Au1 Ba5 172.58(3) 2_646 4_565 ?
Ba2 Au1 Ba5 109.733(17) . 4_565 ?
As15 Au1 Ba3 70.84(3) . 2_646 ?
As6 Au1 Ba3 177.11(3) . 2_646 ?
As13 Au1 Ba3 63.12(3) 4_565 2_646 ?
As2 Au1 Ba3 73.18(3) 2_646 2_646 ?
Ba2 Au1 Ba3 107.524(14) . 2_646 ?
Ba5 Au1 Ba3 112.280(17) 4_565 2_646 ?
As15 Au1 Ba4 73.07(3) . 2_646 ?
As6 Au1 Ba4 73.05(3) . 2_646 ?
As13 Au1 Ba4 170.50(3) 4_565 2_646 ?
As2 Au1 Ba4 60.52(3) 2_646 2_646 ?
Ba2 Au1 Ba4 104.957(14) . 2_646 ?
Ba5 Au1 Ba4 112.241(17) 4_565 2_646 ?
Ba3 Au1 Ba4 109.745(17) 2_646 2_646 ?
As4 Au2 As10 107.20(4) . . ?
As4 Au2 As11 129.15(4) . 4_565 ?
As10 Au2 As11 107.51(4) . 4_565 ?
As4 Au2 As14 101.92(4) . . ?
As10 Au2 As14 104.50(4) . . ?
As11 Au2 As14 104.00(4) 4_565 . ?
As4 Au2 Ba4 77.56(3) . 3_666 ?
As10 Au2 Ba4 81.54(3) . 3_666 ?
As11 Au2 Ba4 72.13(3) 4_565 3_666 ?
As14 Au2 Ba4 173.72(3) . 3_666 ?
As4 Au2 Ba1 161.96(3) . 2_656 ?
As10 Au2 Ba1 66.98(3) . 2_656 ?
As11 Au2 Ba1 68.06(2) 4_565 2_656 ?
As14 Au2 Ba1 64.90(2) . 2_656 ?
Ba4 Au2 Ba1 116.940(16) 3_666 2_656 ?
As4 Au2 Ba5 71.37(3) . 4_565 ?
As10 Au2 Ba5 178.50(3) . 4_565 ?
As11 Au2 Ba5 73.33(3) 4_565 4_565 ?
As14 Au2 Ba5 76.39(3) . 4_565 ?
Ba4 Au2 Ba5 97.611(18) 3_666 4_565 ?
Ba1 Au2 Ba5 114.523(16) 2_656 4_565 ?
As8 Au3 As2 129.57(4) . 3_766 ?
As8 Au3 As1 110.93(4) . 3_666 ?
As2 Au3 As1 106.93(4) 3_766 3_666 ?
As8 Au3 As7 101.71(4) . 4_565 ?
As2 Au3 As7 103.07(4) 3_766 4_565 ?
As1 Au3 As7 100.20(4) 3_666 4_565 ?
As8 Au3 Ba4 76.58(3) . . ?
As2 Au3 Ba4 73.27(3) 3_766 . ?
As1 Au3 Ba4 87.14(3) 3_666 . ?
As7 Au3 Ba4 172.55(3) 4_565 . ?
As8 Au3 Ba4 72.13(3) . 3_766 ?
As2 Au3 Ba4 72.19(3) 3_766 3_766 ?
As1 Au3 Ba4 175.84(3) 3_666 3_766 ?
As7 Au3 Ba4 76.20(3) 4_565 3_766 ?
Ba4 Au3 Ba4 96.410(18) . 3_766 ?
As8 Au3 Ba2 162.36(3) . 2_655 ?
As2 Au3 Ba2 66.68(3) 3_766 2_655 ?
As1 Au3 Ba2 63.84(3) 3_666 2_655 ?
As7 Au3 Ba2 64.44(3) 4_565 2_655 ?
Ba4 Au3 Ba2 118.579(16) . 2_655 ?
Ba4 Au3 Ba2 112.375(16) 3_766 2_655 ?
As14 Au4 As11 108.23(4) . . ?
As14 Au4 As9 111.20(4) . 4_566 ?
As11 Au4 As9 110.70(4) . 4_566 ?
As14 Au4 As5 108.22(4) . 2_646 ?
As11 Au4 As5 108.46(4) . 2_646 ?
As9 Au4 As5 109.94(4) 4_566 2_646 ?
As14 Au4 Ba1 176.99(3) . . ?
As11 Au4 Ba1 71.24(3) . . ?
As9 Au4 Ba1 71.61(3) 4_566 . ?
As5 Au4 Ba1 69.42(3) 2_646 . ?
As14 Au4 Ba3 74.19(3) . . ?
As11 Au4 Ba3 175.01(3) . . ?
As9 Au4 Ba3 64.33(3) 4_566 . ?
As5 Au4 Ba3 74.41(3) 2_646 . ?
Ba1 Au4 Ba3 106.583(14) . . ?
As14 Au4 Ba5 70.31(3) . 4_565 ?
As11 Au4 Ba5 72.85(3) . 4_565 ?
As9 Au4 Ba5 174.90(3) 4_566 4_565 ?
As5 Au4 Ba5 65.10(3) 2_646 4_565 ?
Ba1 Au4 Ba5 106.796(14) . 4_565 ?
Ba3 Au4 Ba5 112.139(18) . 4_565 ?
As5 Au5 As13 107.69(4) . . ?
As5 Au5 As3 119.67(4) . 3_667 ?
As13 Au5 As3 109.50(4) . 3_667 ?
As5 Au5 As9 108.70(4) . 2_656 ?
As13 Au5 As9 105.86(4) . 2_656 ?
As3 Au5 As9 104.61(4) 3_667 2_656 ?
As5 Au5 Ba5 72.34(3) . . ?
As13 Au5 Ba5 79.47(3) . . ?
As3 Au5 Ba5 69.94(3) 3_667 . ?
As9 Au5 Ba5 173.63(3) 2_656 . ?
As5 Au5 Ba5 68.83(3) . 3_667 ?
As13 Au5 Ba5 174.11(3) . 3_667 ?
As3 Au5 Ba5 69.45(3) 3_667 3_667 ?
As9 Au5 Ba5 79.93(3) 2_656 3_667 ?
Ba5 Au5 Ba5 94.833(16) . 3_667 ?
As5 Au5 Ba3 76.72(3) . 2_656 ?
As13 Au5 Ba3 63.59(3) . 2_656 ?
As3 Au5 Ba3 163.50(3) 3_667 2_656 ?
As9 Au5 Ba3 65.46(3) 2_656 2_656 ?
Ba5 Au5 Ba3 120.631(19) . 2_656 ?
Ba5 Au5 Ba3 119.018(18) 3_667 2_656 ?
As5 Au5 Ba3 164.55(3) . 3_667 ?
As13 Au5 Ba3 64.31(3) . 3_667 ?
As3 Au5 Ba3 75.77(3) 3_667 3_667 ?
As9 Au5 Ba3 63.70(3) 2_656 3_667 ?
Ba5 Au5 Ba3 116.820(18) . 3_667 ?
Ba5 Au5 Ba3 120.225(18) 3_667 3_667 ?
Ba3 Au5 Ba3 87.831(14) 2_656 3_667 ?
As4 Au6 As6 133.32(4) . 4_566 ?
As4 Au6 As12 105.44(4) . 1_455 ?
As6 Au6 As12 105.19(4) 4_566 1_455 ?
As4 Au6 As1 101.91(4) . . ?
As6 Au6 As1 104.58(4) 4_566 . ?
As12 Au6 As1 102.86(4) 1_455 . ?
As4 Au6 Ba4 79.88(3) . 2_646 ?
As6 Au6 Ba4 73.10(3) 4_566 2_646 ?
As12 Au6 Ba4 77.97(3) 1_455 2_646 ?
As1 Au6 Ba4 177.68(3) . 2_646 ?
As4 Au6 Ba5 80.20(3) . . ?
As6 Au6 Ba5 69.81(3) 4_566 . ?
As12 Au6 Ba5 174.31(3) 1_455 . ?
As1 Au6 Ba5 76.34(3) . . ?
Ba4 Au6 Ba5 102.624(19) 2_646 . ?
As4 Au6 Ba2 159.42(3) . 2_556 ?
As6 Au6 Ba2 67.01(2) 4_566 2_556 ?
As12 Au6 Ba2 65.51(2) 1_455 2_556 ?
As1 Au6 Ba2 64.48(2) . 2_556 ?
Ba4 Au6 Ba2 114.209(16) 2_646 2_556 ?
Ba5 Au6 Ba2 109.411(16) . 2_556 ?
As8 Au7 As13 127.69(4) . 2_646 ?
As8 Au7 As7 107.41(4) . . ?
As13 Au7 As7 104.19(4) 2_646 . ?
As8 Au7 As12 103.50(4) . 4_565 ?
As13 Au7 As12 105.70(4) 2_646 4_565 ?
As7 Au7 As12 106.99(4) . 4_565 ?
As8 Au7 Ba3 77.85(3) . . ?
As13 Au7 Ba3 69.45(3) 2_646 . ?
As7 Au7 Ba3 77.76(3) . . ?
As12 Au7 Ba3 174.16(3) 4_565 . ?
As8 Au7 Ba2 163.59(3) . 1_655 ?
As13 Au7 Ba2 68.54(3) 2_646 1_655 ?
As7 Au7 Ba2 66.30(2) . 1_655 ?
As12 Au7 Ba2 65.98(2) 4_565 1_655 ?
Ba3 Au7 Ba2 113.950(15) . 1_655 ?
As8 Au7 Ba3 75.24(3) . 4_565 ?
As13 Au7 Ba3 71.02(3) 2_646 4_565 ?
As7 Au7 Ba3 175.01(3) . 4_565 ?
As12 Au7 Ba3 76.12(3) 4_565 4_565 ?
Ba3 Au7 Ba3 98.91(2) . 4_565 ?
Ba2 Au7 Ba3 112.300(15) 1_655 4_565 ?
As8 Au7 Ba4 61.69(3) . 3_766 ?
As13 Au7 Ba4 170.08(3) 2_646 3_766 ?
As7 Au7 Ba4 73.33(3) . 3_766 ?
As12 Au7 Ba4 66.63(3) 4_565 3_766 ?
Ba3 Au7 Ba4 118.561(18) . 3_766 ?
Ba2 Au7 Ba4 101.959(14) 1_655 3_766 ?
Ba3 Au7 Ba4 111.630(18) 4_565 3_766 ?
As9 Au8 As8 132.39(4) . . ?
As9 Au8 As15 107.89(4) . 2_656 ?
As8 Au8 As15 103.68(4) . 2_656 ?
As9 Au8 As10 107.67(4) . 3_666 ?
As8 Au8 As10 99.30(4) . 3_666 ?
As15 Au8 As10 102.10(4) 2_656 3_666 ?
As9 Au8 Ba3 72.63(3) . . ?
As8 Au8 Ba3 78.34(3) . . ?
As15 Au8 Ba3 80.91(3) 2_656 . ?
As10 Au8 Ba3 176.60(3) 3_666 . ?
As9 Au8 Ba3 72.81(3) . 4_565 ?
As8 Au8 Ba3 77.03(3) . 4_565 ?
As15 Au8 Ba3 177.76(3) 2_656 4_565 ?
As10 Au8 Ba3 75.67(3) 3_666 4_565 ?
Ba3 Au8 Ba3 101.325(13) . 4_565 ?
As9 Au8 Ba1 69.41(3) . 2_656 ?
As8 Au8 Ba1 158.06(3) . 2_656 ?
As15 Au8 Ba1 65.24(3) 2_656 2_656 ?
As10 Au8 Ba1 66.73(2) 3_666 2_656 ?
Ba3 Au8 Ba1 116.257(15) . 2_656 ?
Ba3 Au8 Ba1 113.362(16) 4_565 2_656 ?
As14 Ba1 As14 180.0 4_566 2_646 ?
As14 Ba1 As15 108.55(2) 4_566 . ?
As14 Ba1 As15 71.45(2) 2_646 . ?
As14 Ba1 As15 71.45(2) 4_566 3_657 ?
As14 Ba1 As15 108.55(2) 2_646 3_657 ?
As15 Ba1 As15 180.00(3) . 3_657 ?
As14 Ba1 Au4 69.65(2) 4_566 . ?
As14 Ba1 Au4 110.35(2) 2_646 . ?
As15 Ba1 Au4 70.170(18) . . ?
As15 Ba1 Au4 109.829(19) 3_657 . ?
As14 Ba1 Au4 110.35(2) 4_566 3_657 ?
As14 Ba1 Au4 69.65(2) 2_646 3_657 ?
As15 Ba1 Au4 109.830(18) . 3_657 ?
As15 Ba1 Au4 70.171(19) 3_657 3_657 ?
Au4 Ba1 Au4 180.000(14) . 3_657 ?
As14 Ba1 As5 70.46(2) 4_566 4_566 ?
As14 Ba1 As5 109.54(2) 2_646 4_566 ?
As15 Ba1 As5 109.59(3) . 4_566 ?
As15 Ba1 As5 70.41(3) 3_657 4_566 ?
Au4 Ba1 As5 137.290(18) . 4_566 ?
Au4 Ba1 As5 42.710(18) 3_657 4_566 ?
As14 Ba1 As5 109.54(2) 4_566 2_646 ?
As14 Ba1 As5 70.46(2) 2_646 2_646 ?
As15 Ba1 As5 70.41(3) . 2_646 ?
As15 Ba1 As5 109.59(3) 3_657 2_646 ?
Au4 Ba1 As5 42.710(18) . 2_646 ?
Au4 Ba1 As5 137.290(18) 3_657 2_646 ?
As5 Ba1 As5 180.0 4_566 2_646 ?
As14 Ba1 As10 71.06(2) 4_566 4_566 ?
As14 Ba1 As10 108.94(2) 2_646 4_566 ?
As15 Ba1 As10 70.54(3) . 4_566 ?
As15 Ba1 As10 109.46(3) 3_657 4_566 ?
Au4 Ba1 As10 109.682(19) . 4_566 ?
Au4 Ba1 As10 70.318(19) 3_657 4_566 ?
As5 Ba1 As10 41.40(3) 4_566 4_566 ?
As5 Ba1 As10 138.60(3) 2_646 4_566 ?
As14 Ba1 As10 108.94(2) 4_566 2_646 ?
As14 Ba1 As10 71.06(2) 2_646 2_646 ?
As15 Ba1 As10 109.46(3) . 2_646 ?
As15 Ba1 As10 70.54(3) 3_657 2_646 ?
Au4 Ba1 As10 70.318(19) . 2_646 ?
Au4 Ba1 As10 109.682(19) 3_657 2_646 ?
As5 Ba1 As10 138.60(3) 4_566 2_646 ?
As5 Ba1 As10 41.40(3) 2_646 2_646 ?
As10 Ba1 As10 180.0 4_566 2_646 ?
As14 Ba1 As3 137.94(2) 4_566 2_646 ?
As14 Ba1 As3 42.06(2) 2_646 2_646 ?
As15 Ba1 As3 42.33(2) . 2_646 ?
As15 Ba1 As3 137.67(2) 3_657 2_646 ?
Au4 Ba1 As3 71.079(18) . 2_646 ?
Au4 Ba1 As3 108.921(18) 3_657 2_646 ?
As5 Ba1 As3 138.51(2) 4_566 2_646 ?
As5 Ba1 As3 41.49(2) 2_646 2_646 ?
As10 Ba1 As3 109.55(3) 4_566 2_646 ?
As10 Ba1 As3 70.45(3) 2_646 2_646 ?
As14 Ba1 As3 42.06(2) 4_566 4_566 ?
As14 Ba1 As3 137.94(2) 2_646 4_566 ?
As15 Ba1 As3 137.67(2) . 4_566 ?
As15 Ba1 As3 42.33(2) 3_657 4_566 ?
Au4 Ba1 As3 108.921(18) . 4_566 ?
Au4 Ba1 As3 71.079(18) 3_657 4_566 ?
As5 Ba1 As3 41.49(2) 4_566 4_566 ?
As5 Ba1 As3 138.51(2) 2_646 4_566 ?
As10 Ba1 As3 70.45(3) 4_566 4_566 ?
As10 Ba1 As3 109.55(3) 2_646 4_566 ?
As3 Ba1 As3 180.0 2_646 4_566 ?
Au1 Ba2 Au1 180.0 . 3_556 ?
Au1 Ba2 As1 68.87(2) . 4_565 ?
Au1 Ba2 As1 111.13(2) 3_556 4_565 ?
Au1 Ba2 As1 111.13(2) . 2_546 ?
Au1 Ba2 As1 68.87(2) 3_556 2_546 ?
As1 Ba2 As1 180.0 4_565 2_546 ?
Au1 Ba2 As12 108.994(19) . 4_465 ?
Au1 Ba2 As12 71.005(19) 3_556 4_465 ?
As1 Ba2 As12 70.84(2) 4_565 4_465 ?
As1 Ba2 As12 109.16(2) 2_546 4_465 ?
Au1 Ba2 As12 71.006(19) . 2_646 ?
Au1 Ba2 As12 108.995(19) 3_556 2_646 ?
As1 Ba2 As12 109.16(2) 4_565 2_646 ?
As1 Ba2 As12 70.84(2) 2_546 2_646 ?
As12 Ba2 As12 180.0 4_465 2_646 ?
Au1 Ba2 As7 109.221(19) . 3_656 ?
Au1 Ba2 As7 70.779(19) 3_556 3_656 ?
As1 Ba2 As7 69.61(2) 4_565 3_656 ?
As1 Ba2 As7 110.39(2) 2_546 3_656 ?
As12 Ba2 As7 107.87(3) 4_465 3_656 ?
As12 Ba2 As7 72.13(3) 2_646 3_656 ?
Au1 Ba2 As7 70.779(19) . 1_455 ?
Au1 Ba2 As7 109.221(19) 3_556 1_455 ?
As1 Ba2 As7 110.39(2) 4_565 1_455 ?
As1 Ba2 As7 69.61(2) 2_546 1_455 ?
As12 Ba2 As7 72.13(3) 4_465 1_455 ?
As12 Ba2 As7 107.87(3) 2_646 1_455 ?
As7 Ba2 As7 180.0 3_656 1_455 ?
Au1 Ba2 As6 42.372(18) . . ?
Au1 Ba2 As6 137.627(18) 3_556 . ?
As1 Ba2 As6 70.78(2) 4_565 . ?
As1 Ba2 As6 109.22(2) 2_546 . ?
As12 Ba2 As6 70.19(3) 4_465 . ?
As12 Ba2 As6 109.81(3) 2_646 . ?
As7 Ba2 As6 138.28(2) 3_656 . ?
As7 Ba2 As6 41.72(2) 1_455 . ?
Au1 Ba2 As6 137.629(18) . 3_556 ?
Au1 Ba2 As6 42.372(18) 3_556 3_556 ?
As1 Ba2 As6 109.22(2) 4_565 3_556 ?
As1 Ba2 As6 70.78(2) 2_546 3_556 ?
As12 Ba2 As6 109.81(3) 4_465 3_556 ?
As12 Ba2 As6 70.19(3) 2_646 3_556 ?
As7 Ba2 As6 41.72(2) 3_656 3_556 ?
As7 Ba2 As6 138.28(2) 1_455 3_556 ?
As6 Ba2 As6 180.0 . 3_556 ?
Au1 Ba2 As2 137.237(18) . 4_465 ?
Au1 Ba2 As2 42.763(18) 3_556 4_465 ?
As1 Ba2 As2 71.21(3) 4_565 4_465 ?
As1 Ba2 As2 108.79(3) 2_546 4_465 ?
As12 Ba2 As2 41.59(2) 4_465 4_465 ?
As12 Ba2 As2 138.41(2) 2_646 4_465 ?
As7 Ba2 As2 69.38(2) 3_656 4_465 ?
As7 Ba2 As2 110.62(2) 1_455 4_465 ?
As6 Ba2 As2 109.20(2) . 4_465 ?
As6 Ba2 As2 70.80(2) 3_556 4_465 ?
Au1 Ba2 As2 42.763(18) . 2_646 ?
Au1 Ba2 As2 137.237(18) 3_556 2_646 ?
As1 Ba2 As2 108.79(3) 4_565 2_646 ?
As1 Ba2 As2 71.21(3) 2_546 2_646 ?
As12 Ba2 As2 138.41(2) 4_465 2_646 ?
As12 Ba2 As2 41.59(2) 2_646 2_646 ?
As7 Ba2 As2 110.62(2) 3_656 2_646 ?
As7 Ba2 As2 69.38(2) 1_455 2_646 ?
As6 Ba2 As2 70.80(2) . 2_646 ?
As6 Ba2 As2 109.20(2) 3_556 2_646 ?
As2 Ba2 As2 180.0 4_465 2_646 ?
Au8 Ba3 Au8 161.45(2) . 4_566 ?
Au8 Ba3 Au7 67.022(16) . . ?
Au8 Ba3 Au7 128.55(2) 4_566 . ?
Au8 Ba3 As13 81.55(2) . 2_646 ?
Au8 Ba3 As13 104.01(3) 4_566 2_646 ?
Au7 Ba3 As13 41.608(19) . 2_646 ?
Au8 Ba3 Au7 125.40(2) . 4_566 ?
Au8 Ba3 Au7 65.831(16) 4_566 4_566 ?
Au7 Ba3 Au7 101.21(2) . 4_566 ?
As13 Ba3 Au7 125.77(3) 2_646 4_566 ?
Au8 Ba3 As9 40.275(19) . . ?
Au8 Ba3 As9 124.87(3) 4_566 . ?
Au7 Ba3 As9 83.04(2) . . ?
As13 Ba3 As9 68.51(3) 2_646 . ?
Au7 Ba3 As9 162.05(3) 4_566 . ?
Au8 Ba3 As9 122.73(3) . 4_566 ?
Au8 Ba3 As9 39.996(19) 4_566 4_566 ?
Au7 Ba3 As9 165.92(3) . 4_566 ?
As13 Ba3 As9 126.09(3) 2_646 4_566 ?
Au7 Ba3 As9 81.49(2) 4_566 4_566 ?
As9 Ba3 As9 98.66(3) . 4_566 ?
Au8 Ba3 As13 100.42(2) . 3_667 ?
Au8 Ba3 As13 79.43(2) 4_566 3_667 ?
Au7 Ba3 As13 123.77(3) . 3_667 ?
As13 Ba3 As13 163.23(4) 2_646 3_667 ?
Au7 Ba3 As13 40.292(19) 4_566 3_667 ?
As9 Ba3 As13 123.32(3) . 3_667 ?
As9 Ba3 As13 66.87(3) 4_566 3_667 ?
Au8 Ba3 As10 135.53(3) . 2_646 ?
Au8 Ba3 As10 40.912(19) 4_566 2_646 ?
Au7 Ba3 As10 99.98(2) . 2_646 ?
As13 Ba3 As10 64.74(3) 2_646 2_646 ?
Au7 Ba3 As10 98.36(2) 4_566 2_646 ?
As9 Ba3 As10 98.03(3) . 2_646 ?
As9 Ba3 As10 65.94(2) 4_566 2_646 ?
As13 Ba3 As10 120.34(3) 3_667 2_646 ?
Au8 Ba3 As8 158.66(3) . 4_566 ?
Au8 Ba3 As8 39.125(18) 4_566 4_566 ?
Au7 Ba3 As8 99.12(2) . 4_566 ?
As13 Ba3 As8 98.94(3) 2_646 4_566 ?
Au7 Ba3 As8 38.587(18) 4_566 4_566 ?
As9 Ba3 As8 158.60(3) . 4_566 ?
As9 Ba3 As8 74.24(3) 4_566 4_566 ?
As13 Ba3 As8 73.14(3) 3_667 4_566 ?
As10 Ba3 As8 60.58(2) 2_646 4_566 ?
Au8 Ba3 Au5 73.370(17) . 2_646 ?
Au8 Ba3 Au5 99.429(18) 4_566 2_646 ?
Au7 Ba3 Au5 75.038(17) . 2_646 ?
As13 Ba3 Au5 39.57(2) 2_646 2_646 ?
Au7 Ba3 Au5 158.40(2) 4_566 2_646 ?
As9 Ba3 Au5 39.549(19) . 2_646 ?
As9 Ba3 Au5 97.30(2) 4_566 2_646 ?
As13 Ba3 Au5 156.95(3) 3_667 2_646 ?
As10 Ba3 Au5 62.16(2) 2_646 2_646 ?
As8 Ba3 Au5 120.20(2) 4_566 2_646 ?
Au8 Ba3 Au4 97.632(18) . . ?
Au8 Ba3 Au4 64.290(14) 4_566 . ?
Au7 Ba3 Au4 136.35(2) . . ?
As13 Ba3 Au4 97.69(2) 2_646 . ?
Au7 Ba3 Au4 119.64(2) 4_566 . ?
As9 Ba3 Au4 63.07(2) . . ?
As9 Ba3 Au4 38.19(2) 4_566 . ?
As13 Ba3 Au4 98.53(2) 3_667 . ?
As10 Ba3 Au4 61.644(19) 2_646 . ?
As8 Ba3 Au4 103.41(2) 4_566 . ?
Au5 Ba3 Au4 61.328(14) 2_646 . ?
Au3 Ba4 Au6 161.50(3) . 2_656 ?
Au3 Ba4 Au3 83.590(18) . 3_766 ?
Au6 Ba4 Au3 106.07(2) 2_656 3_766 ?
Au3 Ba4 Au2 95.416(19) . 3_666 ?
Au6 Ba4 Au2 80.612(16) 2_656 3_666 ?
Au3 Ba4 Au2 160.71(2) 3_766 3_666 ?
Au3 Ba4 As8 74.37(2) . 3_766 ?
Au6 Ba4 As8 102.10(2) 2_656 3_766 ?
Au3 Ba4 As8 41.67(2) 3_766 3_766 ?
Au2 Ba4 As8 156.01(3) 3_666 3_766 ?
Au3 Ba4 As2 72.05(2) . . ?
Au6 Ba4 As2 125.62(3) 2_656 . ?
Au3 Ba4 As2 41.685(19) 3_766 . ?
Au2 Ba4 As2 119.73(3) 3_666 . ?
As8 Ba4 As2 78.39(3) 3_766 . ?
Au3 Ba4 As2 41.791(19) . 3_766 ?
Au6 Ba4 As2 125.57(3) 2_656 3_766 ?
Au3 Ba4 As2 71.43(2) 3_766 3_766 ?
Au2 Ba4 As2 119.89(3) 3_666 3_766 ?
As8 Ba4 As2 39.73(3) 3_766 3_766 ?
As2 Ba4 As2 89.43(3) . 3_766 ?
Au3 Ba4 As6 119.97(3) . 3_666 ?
Au6 Ba4 As6 41.82(2) 2_656 3_666 ?
Au3 Ba4 As6 128.96(3) 3_766 3_666 ?
Au2 Ba4 As6 67.96(2) 3_666 3_666 ?
As8 Ba4 As6 97.94(3) 3_766 3_666 ?
As2 Ba4 As6 166.32(3) . 3_666 ?
As2 Ba4 As6 96.09(3) 3_766 3_666 ?
Au3 Ba4 As11 120.27(3) . 2_656 ?
Au6 Ba4 As11 67.67(2) 2_656 2_656 ?
Au3 Ba4 As11 124.26(3) 3_766 2_656 ?
Au2 Ba4 As11 40.83(2) 3_666 2_656 ?
As8 Ba4 As11 161.51(3) 3_766 2_656 ?
As2 Ba4 As11 94.87(3) . 2_656 ?
As2 Ba4 As11 158.55(3) 3_766 2_656 ?
As6 Ba4 As11 84.54(3) 3_666 2_656 ?
Au3 Ba4 As8 40.767(19) . . ?
Au6 Ba4 As8 156.97(3) 2_656 . ?
Au3 Ba4 As8 72.07(2) 3_766 . ?
Au2 Ba4 As8 94.60(2) 3_666 . ?
As8 Ba4 As8 91.43(3) 3_766 . ?
As2 Ba4 As8 38.92(3) . . ?
As2 Ba4 As8 76.35(3) 3_766 . ?
As6 Ba4 As8 154.73(3) 3_666 . ?
As11 Ba4 As8 93.95(3) 2_656 . ?
Au3 Ba4 As7 125.19(3) . 2_756 ?
Au6 Ba4 As7 66.25(2) 2_656 2_756 ?
Au3 Ba4 As7 41.609(19) 3_766 2_756 ?
Au2 Ba4 As7 135.16(3) 3_666 2_756 ?
As8 Ba4 As7 64.75(3) 3_766 2_756 ?
As2 Ba4 As7 65.44(3) . 2_756 ?
As2 Ba4 As7 104.11(3) 3_766 2_756 ?
As6 Ba4 As7 101.01(3) 3_666 2_756 ?
As11 Ba4 As7 96.77(3) 2_656 2_756 ?
As8 Ba4 As7 104.21(3) . 2_756 ?
Au3 Ba4 As12 138.65(3) . 2_756 ?
Au6 Ba4 As12 40.620(19) 2_656 2_756 ?
Au3 Ba4 As12 68.07(2) 3_766 2_756 ?
Au2 Ba4 As12 121.19(2) 3_666 2_756 ?
As8 Ba4 As12 64.40(3) 3_766 2_756 ?
As2 Ba4 As12 101.42(3) . 2_756 ?
As2 Ba4 As12 98.95(3) 3_766 2_756 ?
As6 Ba4 As12 65.41(3) 3_666 2_756 ?
As11 Ba4 As12 100.76(3) 2_656 2_756 ?
As8 Ba4 As12 139.09(3) . 2_756 ?
As7 Ba4 As12 36.58(2) 2_756 2_756 ?
Au6 Ba5 As6 41.96(2) . 4_566 ?
Au6 Ba5 Au5 103.045(19) . . ?
As6 Ba5 Au5 103.27(2) 4_566 . ?
Au6 Ba5 Au2 78.980(16) . 4_566 ?
As6 Ba5 Au2 68.28(2) 4_566 4_566 ?
Au5 Ba5 Au2 165.31(2) . 4_566 ?
Au6 Ba5 As3 130.25(3) . 3_667 ?
As6 Ba5 As3 103.35(3) 4_566 3_667 ?
Au5 Ba5 As3 40.80(2) . 3_667 ?
Au2 Ba5 As3 127.52(3) 4_566 3_667 ?
Au6 Ba5 As4 73.33(2) . 4_566 ?
As6 Ba5 As4 39.24(2) 4_566 4_566 ?
Au5 Ba5 As4 126.15(3) . 4_566 ?
Au2 Ba5 As4 40.016(18) 4_566 4_566 ?
As3 Ba5 As4 100.33(3) 3_667 4_566 ?
Au6 Ba5 As5 166.48(3) . 3_667 ?
As6 Ba5 As5 125.43(3) 4_566 3_667 ?
Au5 Ba5 As5 73.11(2) . 3_667 ?
Au2 Ba5 As5 101.48(2) 4_566 3_667 ?
As3 Ba5 As5 39.59(2) 3_667 3_667 ?
As4 Ba5 As5 98.18(3) 4_566 3_667 ?
Au6 Ba5 As5 99.80(3) . . ?
As6 Ba5 As5 126.82(3) 4_566 . ?
Au5 Ba5 As5 39.708(19) . . ?
Au2 Ba5 As5 154.87(3) 4_566 . ?
As3 Ba5 As5 72.37(3) 3_667 . ?
As4 Ba5 As5 163.57(3) 4_566 . ?
As5 Ba5 As5 85.51(3) 3_667 . ?
Au6 Ba5 As3 120.25(3) . . ?
As6 Ba5 As3 161.04(3) 4_566 . ?
Au5 Ba5 As3 71.51(2) . . ?
Au2 Ba5 As3 120.38(2) 4_566 . ?
As3 Ba5 As3 84.71(3) 3_667 . ?
As4 Ba5 As3 157.05(3) 4_566 . ?
As5 Ba5 As3 71.41(3) 3_667 . ?
As5 Ba5 As3 38.93(2) . . ?
Au6 Ba5 Au1 66.902(15) . 4_566 ?
As6 Ba5 Au1 39.963(19) 4_566 4_566 ?
Au5 Ba5 Au1 65.599(14) . 4_566 ?
Au2 Ba5 Au1 102.788(19) 4_566 4_566 ?
As3 Ba5 Au1 66.37(2) 3_667 4_566 ?
As4 Ba5 Au1 63.99(2) 4_566 4_566 ?
As5 Ba5 Au1 100.05(2) 3_667 4_566 ?
As5 Ba5 Au1 99.63(2) . 4_566 ?
As3 Ba5 Au1 136.80(2) . 4_566 ?
Au6 Ba5 As11 66.00(2) . . ?
As6 Ba5 As11 84.39(3) 4_566 . ?
Au5 Ba5 As11 153.94(3) . . ?
Au2 Ba5 As11 40.03(2) 4_566 . ?
As3 Ba5 As11 161.81(3) 3_667 . ?
As4 Ba5 As11 75.10(3) 4_566 . ?
As5 Ba5 As11 122.80(3) 3_667 . ?
As5 Ba5 As11 116.34(3) . . ?
As3 Ba5 As11 93.10(3) . . ?
Au1 Ba5 As11 124.13(2) 4_566 . ?
Au6 Ba5 Au5 154.60(2) . 3_667 ?
As6 Ba5 Au5 159.64(3) 4_566 3_667 ?
Au5 Ba5 Au5 85.168(16) . 3_667 ?
Au2 Ba5 Au5 99.195(18) 4_566 3_667 ?
As3 Ba5 Au5 70.85(2) 3_667 3_667 ?
As4 Ba5 Au5 121.22(3) 4_566 3_667 ?
As5 Ba5 Au5 38.923(19) 3_667 3_667 ?
As5 Ba5 Au5 71.09(2) . 3_667 ?
As3 Ba5 Au5 39.291(19) . 3_667 ?
Au1 Ba5 Au5 136.96(2) 4_566 3_667 ?
As11 Ba5 Au5 96.15(2) . 3_667 ?
As10 As1 As13 108.54(5) . . ?
As10 As1 Au3 98.76(5) . 3_666 ?
As13 As1 Au3 112.73(5) . 3_666 ?
As10 As1 Au6 112.65(5) . . ?
As13 As1 Au6 113.71(5) . . ?
Au3 As1 Au6 109.53(4) 3_666 . ?
As10 As1 Ba2 172.59(5) . 2_556 ?
As13 As1 Ba2 72.29(4) . 2_556 ?
Au3 As1 Ba2 74.41(3) 3_666 2_556 ?
Au6 As1 Ba2 72.94(3) . 2_556 ?
As10 As1 Ba5 80.55(4) . . ?
As13 As1 Ba5 76.03(4) . . ?
Au3 As1 Ba5 170.74(4) 3_666 . ?
Au6 As1 Ba5 62.80(3) . . ?
Ba2 As1 Ba5 106.66(3) 2_556 . ?
As8 As2 As12 107.54(5) . . ?
As8 As2 Au3 117.38(5) . 3_766 ?
As12 As2 Au3 107.13(5) . 3_766 ?
As8 As2 Au1 109.16(5) . 2_656 ?
As12 As2 Au1 104.76(5) . 2_656 ?
Au3 As2 Au1 110.08(4) 3_766 2_656 ?
As8 As2 Ba2 169.86(5) . 2_656 ?
As12 As2 Ba2 67.58(4) . 2_656 ?
Au3 As2 Ba2 72.76(3) 3_766 2_656 ?
Au1 As2 Ba2 65.02(3) 2_656 2_656 ?
As8 As2 Ba4 73.69(4) . . ?
As12 As2 Ba4 172.22(5) . . ?
Au3 As2 Ba4 66.12(3) 3_766 . ?
Au1 As2 Ba4 81.73(3) 2_656 . ?
Ba2 As2 Ba4 112.40(3) 2_656 . ?
As8 As2 Ba4 69.77(4) . 3_766 ?
As12 As2 Ba4 82.82(4) . 3_766 ?
Au3 As2 Ba4 64.94(3) 3_766 3_766 ?
Au1 As2 Ba4 172.14(4) 2_656 3_766 ?
Ba2 As2 Ba4 117.20(3) 2_656 3_766 ?
Ba4 As2 Ba4 90.57(3) . 3_766 ?
As5 As3 As14 106.01(5) . . ?
As5 As3 As15 105.49(5) . 2_656 ?
As14 As3 As15 105.65(5) . 2_656 ?
As5 As3 Au5 120.85(5) . 3_667 ?
As14 As3 Au5 112.10(5) . 3_667 ?
As15 As3 Au5 105.61(5) 2_656 3_667 ?
As5 As3 Ba1 68.11(4) . 2_656 ?
As14 As3 Ba1 66.46(4) . 2_656 ?
As15 As3 Ba1 66.41(4) 2_656 2_656 ?
Au5 As3 Ba1 170.15(4) 3_667 2_656 ?
As5 As3 Ba5 71.66(4) . 3_667 ?
As14 As3 Ba5 177.64(5) . 3_667 ?
As15 As3 Ba5 75.55(4) 2_656 3_667 ?
Au5 As3 Ba5 69.26(3) 3_667 3_667 ?
Ba1 As3 Ba5 112.55(3) 2_656 3_667 ?
As5 As3 Ba5 70.13(4) . . ?
As14 As3 Ba5 83.46(4) . . ?
As15 As3 Ba5 170.80(5) 2_656 . ?
Au5 As3 Ba5 71.25(3) 3_667 . ?
Ba1 As3 Ba5 117.54(3) 2_656 . ?
Ba5 As3 Ba5 95.29(3) 3_667 . ?
As6 As4 Au6 108.55(5) . . ?
As6 As4 Au2 109.23(5) . . ?
Au6 As4 Au2 111.49(4) . . ?
As6 As4 As11 108.48(5) . . ?
Au6 As4 As11 105.74(5) . . ?
Au2 As4 As11 113.18(5) . . ?
As6 As4 Ba5 67.17(4) . 4_565 ?
Au6 As4 Ba5 175.04(5) . 4_565 ?
Au2 As4 Ba5 68.61(3) . 4_565 ?
As11 As4 Ba5 78.41(4) . 4_565 ?
As6 As4 Ba4 78.28(4) . 2_646 ?
Au6 As4 Ba4 61.06(3) . 2_646 ?
Au2 As4 Ba4 171.34(4) . 2_646 ?
As11 As4 Ba4 67.01(3) . 2_646 ?
Ba5 As4 Ba4 119.23(3) 4_565 2_646 ?
As10 As5 As3 109.95(5) . . ?
As10 As5 Au5 106.40(5) . . ?
As3 As5 Au5 119.43(5) . . ?
As10 As5 Au4 106.51(5) . 2_656 ?
As3 As5 Au4 108.22(5) . 2_656 ?
Au5 As5 Au4 105.59(4) . 2_656 ?
As10 As5 Ba1 69.64(4) . 2_656 ?
As3 As5 Ba1 70.39(4) . 2_656 ?
Au5 As5 Ba1 170.04(4) . 2_656 ?
Au4 As5 Ba1 67.87(3) 2_656 2_656 ?
As10 As5 Ba5 176.76(5) . 3_667 ?
As3 As5 Ba5 68.74(4) . 3_667 ?
Au5 As5 Ba5 72.25(3) . 3_667 ?
Au4 As5 Ba5 76.73(3) 2_656 3_667 ?
Ba1 As5 Ba5 112.18(3) 2_656 3_667 ?
As10 As5 Ba5 82.28(4) . . ?
As3 As5 Ba5 70.94(4) . . ?
Au5 As5 Ba5 67.96(3) . . ?
Au4 As5 Ba5 170.58(5) 2_656 . ?
Ba1 As5 Ba5 119.44(3) 2_656 . ?
Ba5 As5 Ba5 94.48(3) 3_667 . ?
As4 As6 As7 107.28(5) . 1_455 ?
As4 As6 Au1 106.12(5) . . ?
As7 As6 Au1 105.26(4) 1_455 . ?
As4 As6 Au6 120.27(5) . 4_565 ?
As7 As6 Au6 111.08(5) 1_455 4_565 ?
Au1 As6 Au6 105.74(4) . 4_565 ?
As4 As6 Ba2 167.57(5) . . ?
As7 As6 Ba2 68.00(3) 1_455 . ?
Au1 As6 Ba2 65.57(2) . . ?
Au6 As6 Ba2 71.83(3) 4_565 . ?
As4 As6 Ba5 73.59(4) . 4_565 ?
As7 As6 Ba5 179.13(5) 1_455 4_565 ?
Au1 As6 Ba5 74.53(3) . 4_565 ?
Au6 As6 Ba5 68.23(3) 4_565 4_565 ?
Ba2 As6 Ba5 111.18(3) . 4_565 ?
As4 As6 Ba4 77.39(4) . 3_666 ?
As7 As6 Ba4 81.90(4) 1_455 3_666 ?
Au1 As6 Ba4 170.26(4) . 3_666 ?
Au6 As6 Ba4 65.08(3) 4_565 3_666 ?
Ba2 As6 Ba4 112.39(3) . 3_666 ?
Ba5 As6 Ba4 98.21(3) 4_565 3_666 ?
As12 As7 As6 107.76(5) . 1_655 ?
As12 As7 Au7 106.53(5) . . ?
As6 As7 Au7 107.06(5) 1_655 . ?
As12 As7 Au3 110.02(5) . 4_566 ?
As6 As7 Au3 111.95(5) 1_655 4_566 ?
Au7 As7 Au3 113.22(4) . 4_566 ?
As12 As7 Ba2 176.72(5) . 1_655 ?
As6 As7 Ba2 70.27(3) 1_655 1_655 ?
Au7 As7 Ba2 71.94(3) . 1_655 ?
Au3 As7 Ba2 73.26(3) 4_566 1_655 ?
As12 As7 Ba4 72.39(4) . 2_746 ?
As6 As7 Ba4 79.02(4) 1_655 2_746 ?
Au7 As7 Ba4 173.73(4) . 2_746 ?
Au3 As7 Ba4 62.19(3) 4_566 2_746 ?
Ba2 As7 Ba4 109.45(3) 1_655 2_746 ?
As2 As8 Au7 107.44(5) . . ?
As2 As8 Au8 109.45(5) . . ?
Au7 As8 Au8 103.47(4) . . ?
As2 As8 Au3 112.64(5) . . ?
Au7 As8 Au3 113.45(4) . . ?
Au8 As8 Au3 109.95(4) . . ?
As2 As8 Ba4 70.50(4) . 3_766 ?
Au7 As8 Ba4 80.94(3) . 3_766 ?
Au8 As8 Ba4 175.23(4) . 3_766 ?
Au3 As8 Ba4 66.19(3) . 3_766 ?
As2 As8 Ba4 67.39(3) . . ?
Au7 As8 Ba4 169.43(4) . . ?
Au8 As8 Ba4 87.06(3) . . ?
Au3 As8 Ba4 62.65(3) . . ?
Ba4 As8 Ba4 88.57(3) 3_766 . ?
As2 As8 Ba3 167.71(5) . 4_565 ?
Au7 As8 Ba3 66.17(3) . 4_565 ?
Au8 As8 Ba3 63.84(3) . 4_565 ?
Au3 As8 Ba3 79.65(3) . 4_565 ?
Ba4 As8 Ba3 117.11(3) 3_766 4_565 ?
Ba4 As8 Ba3 120.65(3) . 4_565 ?
As14 As9 Au8 107.68(5) . . ?
As14 As9 Au4 104.43(5) . 4_565 ?
Au8 As9 Au4 107.27(4) . 4_565 ?
As14 As9 Au5 106.01(5) . 2_646 ?
Au8 As9 Au5 123.52(4) . 2_646 ?
Au4 As9 Au5 106.43(4) 4_565 2_646 ?
As14 As9 Ba1 66.26(3) . 2_656 ?
Au8 As9 Ba1 70.27(3) . 2_656 ?
Au4 As9 Ba1 66.42(2) 4_565 2_656 ?
Au5 As9 Ba1 166.20(4) 2_646 2_656 ?
As14 As9 Ba3 81.25(4) . . ?
Au8 As9 Ba3 67.09(3) . . ?
Au4 As9 Ba3 173.25(4) 4_565 . ?
Au5 As9 Ba3 74.99(3) 2_646 . ?
Ba1 As9 Ba3 113.57(3) 2_656 . ?
As14 As9 Ba3 174.87(5) . 4_565 ?
Au8 As9 Ba3 67.19(3) . 4_565 ?
Au4 As9 Ba3 77.48(3) 4_565 4_565 ?
Au5 As9 Ba3 77.74(3) 2_646 4_565 ?
Ba1 As9 Ba3 110.78(3) 2_656 4_565 ?
Ba3 As9 Ba3 96.56(3) . 4_565 ?
As1 As10 As5 107.00(6) . . ?
As1 As10 Au2 104.93(5) . . ?
As5 As10 Au2 109.03(5) . . ?
As1 As10 Au8 117.14(5) . 3_666 ?
As5 As10 Au8 108.59(5) . 3_666 ?
Au2 As10 Au8 109.88(4) . 3_666 ?
As1 As10 Ba1 172.44(5) . 2_656 ?
As5 As10 Ba1 68.96(4) . 2_656 ?
Au2 As10 Ba1 71.30(3) . 2_656 ?
Au8 As10 Ba1 70.42(3) 3_666 2_656 ?
As1 As10 Ba3 76.12(4) . 2_656 ?
As5 As10 Ba3 77.70(4) . 2_656 ?
Au2 As10 Ba3 172.20(4) . 2_656 ?
Au8 As10 Ba3 63.42(3) 3_666 2_656 ?
Ba1 As10 Ba3 108.54(3) 2_656 2_656 ?
As15 As11 Au4 106.20(5) . . ?
As15 As11 As4 108.43(5) . . ?
Au4 As11 As4 104.88(5) . . ?
As15 As11 Au2 106.60(5) . 4_566 ?
Au4 As11 Au2 107.80(4) . 4_566 ?
As4 As11 Au2 121.98(5) . 4_566 ?
As15 As11 Ba1 66.79(3) . . ?
Au4 As11 Ba1 66.95(3) . . ?
As4 As11 Ba1 167.50(5) . . ?
Au2 As11 Ba1 70.36(3) 4_566 . ?
As15 As11 Ba4 81.49(4) . 2_646 ?
Au4 As11 Ba4 171.96(4) . 2_646 ?
As4 As11 Ba4 74.22(4) . 2_646 ?
Au2 As11 Ba4 67.04(3) 4_566 2_646 ?
Ba1 As11 Ba4 115.25(3) . 2_646 ?
As15 As11 Ba5 172.64(5) . . ?
Au4 As11 Ba5 79.29(3) . . ?
As4 As11 Ba5 74.24(4) . . ?
Au2 As11 Ba5 66.64(3) 4_566 . ?
Ba1 As11 Ba5 112.01(3) . . ?
Ba4 As11 Ba5 92.85(3) 2_646 . ?
As7 As12 As2 109.07(6) . . ?
As7 As12 Au6 106.68(5) . 1_655 ?
As2 As12 Au6 112.06(5) . 1_655 ?
As7 As12 Au7 109.08(5) . 4_566 ?
As2 As12 Au7 111.11(5) . 4_566 ?
Au6 As12 Au7 108.70(4) 1_655 4_566 ?
As7 As12 Ba2 179.16(5) . 2_656 ?
As2 As12 Ba2 70.82(3) . 2_656 ?
Au6 As12 Ba2 72.66(3) 1_655 2_656 ?
Au7 As12 Ba2 71.68(3) 4_566 2_656 ?
As7 As12 Ba4 71.03(4) . 2_746 ?
As2 As12 Ba4 172.52(5) . 2_746 ?
Au6 As12 Ba4 61.41(3) 1_655 2_746 ?
Au7 As12 Ba4 75.42(3) 4_566 2_746 ?
Ba2 As12 Ba4 108.96(3) 2_656 2_746 ?
As1 As13 Au1 101.44(4) . 4_566 ?
As1 As13 Au7 109.04(5) . 2_656 ?
Au1 As13 Au7 107.62(4) 4_566 2_656 ?
As1 As13 Au5 104.28(5) . . ?
Au1 As13 Au5 104.61(4) 4_566 . ?
Au7 As13 Au5 127.00(4) 2_656 . ?
As1 As13 Ba3 81.47(4) . 2_656 ?
Au1 As13 Ba3 176.19(4) 4_566 2_656 ?
Au7 As13 Ba3 68.94(3) 2_656 2_656 ?
Au5 As13 Ba3 76.85(3) . 2_656 ?
As1 As13 Ba2 66.66(3) . 2_556 ?
Au1 As13 Ba2 64.75(2) 4_566 2_556 ?
Au7 As13 Ba2 70.32(3) 2_656 2_556 ?
Au5 As13 Ba2 162.65(4) . 2_556 ?
Ba3 As13 Ba2 114.69(3) 2_656 2_556 ?
As1 As13 Ba3 177.72(5) . 3_667 ?
Au1 As13 Ba3 79.33(3) 4_566 3_667 ?
Au7 As13 Ba3 68.68(3) 2_656 3_667 ?
Au5 As13 Ba3 77.52(3) . 3_667 ?
Ba3 As13 Ba3 97.67(2) 2_656 3_667 ?
Ba2 As13 Ba3 111.98(3) 2_556 3_667 ?
As9 As14 Au4 108.45(5) . . ?
As9 As14 As3 110.68(5) . . ?
Au4 As14 As3 103.71(5) . . ?
As9 As14 Au2 112.70(5) . . ?
Au4 As14 Au2 110.82(4) . . ?
As3 As14 Au2 110.10(5) . . ?
As9 As14 Ba1 72.83(4) . 2_656 ?
Au4 As14 Ba1 175.05(4) . 2_656 ?
As3 As14 Ba1 71.47(3) . 2_656 ?
Au2 As14 Ba1 72.51(3) . 2_656 ?
As11 As15 Au1 105.98(5) . . ?
As11 As15 As3 111.36(5) . 2_646 ?
Au1 As15 As3 108.48(5) . 2_646 ?
As11 As15 Au8 113.71(5) . 2_646 ?
Au1 As15 Au8 109.88(4) . 2_646 ?
As3 As15 Au8 107.34(5) 2_646 2_646 ?
As11 As15 Ba1 72.26(4) . . ?
Au1 As15 Ba1 177.80(4) . . ?
As3 As15 Ba1 71.25(4) 2_646 . ?
Au8 As15 Ba1 72.20(3) 2_646 . ?

_refine_diff_density_max         2.182
_refine_diff_density_min         -2.361
_refine_diff_density_rms         0.517



_exptl_crystal_recrystallization_method 'Flux growth: CsBr/CsI'
